Analysis of creep properties has traditionally been made with empirical methods involving a number of adjustable parameters. This makes it quite difficult to make predictions outside the range of the original data. In recent years, the author has formulated basic models for prediction of creep properties, covering dislocation, particle and solid solution hardening. These models do not use adjustable parameters. In the present chapter, these models are further developed and utilised. The dislocation mobilities play an important role. The high-temperature climb mobility is extended to low temperatures by taking vacancies generated by plastic deformation into account. This new expression verifies the validity of the combined climb and glide mobility that has been used so far. By assuming that the glide rate is controlled by the climb of the jogs, a dislocation glide mobility is formulated. The role of the mobilities is analysed, and various creep properties are derived. For example, secondary creep rates and strain versus time curves are computed and show good agreement with experimental data.
- creep strain
If metals are exposed to load at high temperatures, a slow deformation called creep takes place. A characteristic feature of creep is that it occurs even when the load is kept constant. This should be contrasted to plastic deformation at ambient temperatures where an increase in the load is needed to generate further plastic strain. Creep in metals has been studied for many decades, and a number of excellent textbooks exist on the subject, see for example [1–4]. A common way of measuring the creep deformation is to apply a fixed load to a specimen and then record its elongation as a function of time. The relative increase in the elongation is referred to as the (creep) strain. Its time derivative is called the creep strain rate. Another important quantity is the stress, i.e. the load divided by the specimen cross section. After sufficient test time, the specimen ruptures. The rupture time and the specimen elongation at rupture are recorded.
A creep test typically shows three stages: primary, secondary and tertiary. During the primary stage, the creep rate is initially high but shows a gradual decrease until it reaches a constant value, which corresponds to the secondary stage. This stage usually takes the longest time. Finally, the creep rate starts to increase. This is the tertiary stage that eventually leads to rupture. The dependence of the creep strain as a function of time is referred to as a creep (strain) curve. Although the described shape of the creep curve is the most common one, there are many variants.
Creep-exposed materials can be found in many types of high-temperature plants, for example, fossil-fired power plants. The desire is to make the materials as strong as possible, and the creep rate low to ensure a long lifetime. The deformation rate is controlled by the movement of the dislocations, i.e. the line defects that are present in large numbers. If the movement of the dislocations is fast, the creep strength is low. To increase the creep strength, the movement of the dislocations must be reduced. Typically, the most efficient way to hinder this movement is to have a high content of other (forest) dislocations. There is a strong interaction between different dislocations. The second most used way of increasing the strength is to introduce particles in the microstructure. Particles or precipitates are a very potent way of raising the strength. A third way is to have elements in solid solution. The difference in size between the solute and the matrix atoms makes it more difficult for the dislocations to move.
Most creep investigations concern metals above half the melting point. The stress dependence of the strain rate in the secondary stage has always generated much interest in creep research because it has been assumed to reflect the operating dislocation mechanism. In Figure 1, such dependence is illustrated for 0.5Cr0.5Mo0.25V steel at 565°C over a wide range of stresses.
The slope of the curve is the creep exponent
In the past, the creep exponent has often been used to identify the operating dislocation mechanisms. For intermediate exponents (3–8), climb of dislocations is in general considered as the operating mechanisms although glide has also been assumed for certain alloy types. This will be discussed below. At high stresses, glide has been suggested as the dominating mechanism. At low creep exponents approaching unity, diffusion creep has been assumed as the main mechanism. The consistent change of operating mechanism with stress has been challenged, see for example .
In recent years, basic creep models have been formulated. With the help of these models, the assumptions mentioned above will be reanalysed in the present chapter.
2. Dislocation model
To understand the creep process, the key quantity is the dislocation density and its variation with time. Models for the dislocation density development during creep have been available for a long time . Recently, these models have been expanded and derived more precisely. We will use the following formulation :
Eq. (1) describes the development of the dislocation density with strain. The first term on the right-hand side is responsible for the generation of dislocations, i.e. work hardening. The two other terms take into account the annihilation of dislocations. The second term gives a strain-controlled recovery, which is called dynamic recovery. The final term is referred to as static recovery. It is time controlled since the strain rate appears in the denominator. The terminology of recovery is not consistent in the literature, which one has to be aware of.
3. Dislocation mobilities
3.1. Climb mobility
The dislocation mobility
where σ is the applied stress. Dislocations can propagate by glide along their slip system or by climb perpendicular to the slip system. The latter process requires emission or absorption of atoms by diffusion, and it is slower than glide. The climb mobility at high temperatures (>0.4
At lower temperatures, the climb rate is influenced by the generation of vacancies due to plastic deformation. A brief derivation of this effect will be given here since it cannot be found in the literature. When a climbing dislocation is forced to move, it will emit or absorb vacancies. When gliding dislocations cut each other, jogs in the form of steps of the length of a Burgers vector are formed on them. The jogs are often sessile and must then climb when they move and hence emit or absorb vacancies.
Mecking and Estrin  have estimated the number of vacancies produced mechanically in a unit volume per unit time as:
The quantities in this equation have been defined above. In  the constant in Eq. (6) was estimated to 0.1. A detailed derivation shows that it is 0.5. The annihilation rate
In deriving Eq. (9), we have also made use of a relation for the self-diffusion coefficient:
where Ω is the atomic volume. It is now assumed that the climb rate is proportional to the total vacancy concentration. This is the same assumption as was made in . The increase in the climb rate
To find the total climb mobility, the expression in Eq. (5) should be multiplied by
3.2. The glide mobility
In a dislocation-free crystal, the glide mobility is very high. Edington measured a mobility of
The basis for the glide mobility is Eq. (12), since the jogs move by climb. However, there is an additional factor. Only a small fraction of each dislocation consists of jogs. Since the jogs move slowly, the forces on the dislocations are concentrated to the jogs. The average distance between jogs can be determined from the dislocation density
where the length of a jog is taken as the length of the Burgers vector. With the help of Taylor’s equation,
where σy being the yield strength, Eq. (13) can be rewritten as
The glide mobility is obtained by multiplying the climb mobility by
Eq. (16) applies to both edge and screw dislocations. With the assumptions considered, the climb and glide mobility are closely related.
3.3. Cross slip mobility
Screw dislocations can change glide plane with the help of cross slip. This can simplify the annihilation of dislocations with opposite signs and thereby contribute to the recovery. Cross slip requires an additional activation energy
where νP is Poisson’s ratio and γSFE is the stacking-fault energy. With stacking-fault energies of 45 mJ/m2 for copper and 166 mJ/m2 for aluminium , the resulting values for
The consequences of the strong temperature dependence in the model for cross slip mobility will be discussed later in Section 6.
3.4. The climb-glide mobility
The results in Sections 3.1–3.3 are new. It has been recognised that the climb mobility in Eq. (5) predicted far too low creep rates at low temperatures and high stresses. It was thought that glide could be the controlling mechanism during these conditions. For this purpose, a combined climb and glide mobility was introduced :
The derivation of Eq. (21) was inspired by the work of Kocks et al. . They gave an empirical expression for the glide mobility. Unfortunately, it involved five unknown parameters and was therefore of little use directly. However, some of the parameters could be fixed by following a procedure due to Nes where an integrated climb and glide mobility was formulated . The remaining parameters could be set with the help of work by Chandler .
Ideally, to describe creep, the fundamental models for the mobilities derived in Sections 3.1–3.3 should be used. However, they are difficult to use directly since
In Figure 2, a continuous set of parameters for temperature and strain rate are used, whereas in Figure 3 experimental values are applied. It can be seen that the enhancement in vacancy concentration due to plastic deformation can fully explain the increase in creep rate in relation to the high-temperature climb mobility.
A second example of the comparison is given in Figure 4 for copper.
4. Secondary creep
4.1. Pure elements
Our understanding of the creep process is largely based on the creep recovery theory . The key feature of this theory is that the recovery rate is sufficiently rapid that the dislocation density can be kept constant during secondary creep. If the dislocation density is continuously rising, the creep deformation will slow down and eventually stop, which is contrary to observations. Thus, there is a balance between the generation and the annihilation of dislocations during creep. If we assume stationary conditions, the strain derivative in Eq. (1) vanishes. The resulting expression for secondary strain rate is
where σdisl is the dislocation stress. σi is an internal stress that can have contributions from the yield strength, solid solution hardening and particle hardening. At low stresses, the mobility
With our present knowledge, the natural assumption is that static recovery is controlled by climb. This is analysed in Section 6. This means that it is the climb mobility in Eq. (12) that should be used in Eq. (24). In addition, we saw in Section 3.4 that the expression for the enhancement factor for the climb mobility
Eq. (24) will now be applied to pure aluminium. For σi, the Peierls stress will be used. Although a Peierls stress is not usually considered to be of importance for fcc alloys, recent studies suggest that this conclusion is not true for Al. With ab initio methods, Shin and Carter found the following value for the Peierls stress of edge dislocation σpe . The value for screw dislocations was much smaller:
At intermediate stresses in Figure 5, the slope of the curves is about 4.5, which is the value of the stress exponent. At higher stresses, the slope increases that is referred to as power-law breakdown. At low stresses, there is also an increase of the stress exponent. This is due to the presence of the internal stress in Eq. (26). It can be seen that the model in Eq. (24) can handle these three regions of the creep rate versus stress curves quite well.
4.2. Solid solution
The presence of elements in solid solution has two effects on the secondary creep rate. It gives rice to a drag stress or a break stress, and it increases the activation energy for creep. The increase in the activation energy is , which is the maximum interaction energy between a dislocation and a solute
where Ω0 is the atomic volume and ε
The use of Eq. (29) is illustrated for Al-Mg alloys in Figure 6. The drag stress is added to the internal stress in Eq. (24). The factor in Eq. (28) is also taken into account which raises the activation energy for creep by the amount , where
In the same way as for pure aluminium, there are three stages of stress dependence. In the middle range of stresses, power-law behaviour is obeyed. At low stresses, there is a slight increase in the creep exponent due to the presence of the Peierls stress that is the same as for pure aluminium. At high stresses, power-law breakdown takes place with an increase in the stress exponent.
The modelling in Figure 6 is based on the climb mobility, so climb is assumed to be the controlling mechanism over the full-stress range. In the literature, it has frequently been assumed that glide is controlling in the middle stress range, see for example . This should be due to a larger effect of solid solution hardening on gliding than on climbing dislocations. This is difficult to understand, since solid solution hardening has about the same effect for both mechanisms . In addition, why there should be transitions in mechanism at low and high stresses is not obvious. Sometimes, it is assumed that the solutes break away from the dislocations at high stresses, but that is predicted to take place at much higher stresses than where the transition takes place . Considering glide as a controlling mechanism is not consistent with the glide mobility in Eq. (16). If that is applied, the experimental results in Figure 6 cannot be reproduced.
For fast diffusion elements such as interstitials, the drag stress according to Eq. (29) is usually negligibly small. Instead, the solutes are locked to the dislocations, and they have to break away to become mobile. The size of the break stress that should be added to the internal stress σi in Eq. (24) is given by [28, 32]
The break stress is proportional to .
From Figure 7, it is obvious that the model can describe the influence of phosphorus on the creep rate quantitatively. No adjustable parameters are used in this figure (or in any other figure in the chapter). For Cu-OFP the creep exponent is about 65 in Figure 7. This demonstrates the validity of Eq. (24) also deep down in the power-law breakdown regime.
5. Creep strain curves
In the primary stage, the creep rate is in most cases larger than in the secondary stage. This is assumed to be due to a lower dislocation density and thereby a lower dislocation stress. The additional driving stress during primary creep becomes 
where σdislstat is the dislocation density during stationary conditions, which is given by the difference between the applied stress σ and the internal stress σi:
The total stress during primary creep is given by
where Eqs. (31) and (32) have been inserted. Eq. (33) gives the stress that should be used in the expression for the secondary creep rate (Eq. (24)) to obtain the general expression for the creep rate:
When the secondary stage is reached, σ = σi + σdisl and are equal to the secondary creep rate, according to Eq. (24) as it should. When σdisl is smaller than its stationary value, the creep rate is higher, which is characteristic for primary creep. The use of Eq. (34) is illustrated in Figure 8. In Figure 8a, a creep strain versus time curve is shown for Cu-OFP. The creep rate versus time for the same case is given in Figure 8b. In the double logarithmic diagram, a straight line is obtained, which is in close agreement with the experimental data. This type of relation that is referred to as the ϕ model is quite frequently observed. It has several different names . It is most well known for 9% Cr steels, see for example . It is evident that Eq. (34) can describe primary creep quite well.
6. Creep recovery theory
At ambient temperatures, for example, in steels, a gradually decreasing creep rate is observed at constant load until the deformation in practice stops completely. This is known as logarithmic creep. In constant strain rate tests, the deformation increases as long as the load is increasing. This behaviour takes work hardening and dynamic recovery into account but not static recovery. The derivation of the expression for the dynamic recovery constant is based on pure glide . It has been suggested many times in the literature that dynamic recovery is controlled by cross slip, see for example [15, 37]. Qualitatively, this might seem logically. Cross slip allows the screw dislocations to annihilate each other, leading to the partial recovery that is characteristic for deformation processes at ambient temperatures in steels. The problem is that the available models for cross slip that were summarised in Section 3.3 give temperature dependencies that are orders of magnitude larger than the observed ones. Unfortunately, we must conclude that we do not understand the role of cross slip at present. In fact, we can model observed dynamic recovery considering just glide.
Most measured creep curves are characterised by a primary, a secondary and a tertiary stage. Work hardening and recovery are continuously taking place. According to the creep recovery theory, there is balance between work hardening and recovery in the secondary stage. Otherwise, there would be either a raise or a decrease in the dislocation density, giving a reduction or increase in the creep rate, respectively. Consequently, the dislocation density must remain approximately unchanged in the secondary stage.
At high temperatures (
At or close to ambient temperatures, several metals give creep curves that have the same general appearance as at high temperatures (
To model creep of alloys, the development of the dislocation density must be known. In recent years, a basic model for the dislocation density has been formulated that fulfils this requirement. Together with models for solid solution and particle hardening, the creep behaviour of many alloys can be described without the use of adjustable parameters.
A new expression for the dislocation climb mobility has been derived. It extends the well-established formula of Hirth and Lothe to lower temperatures by taking the enhanced concentration of vacancies due to plastic deformation into account. The new expression can explain observed creep rates down to near-ambient temperatures.
Assuming that glide of dislocations is controlled by the climb rate of their jogs, an expression for the dislocation glide mobility is formulated. It turns out that the glide rate is always higher than the climb rate. This suggests that climb is rate controlling in dislocation creep. In the chapter, it is illustrated for AlMg alloys that this might apply to class I alloys as well.
It is suggested in the literature that cross slip is the controlling mechanism for dynamic recovery. An expression for the cross slip mobility is set up based on published models for the activation energy of cross slip. However, this expression cannot explain the observed rate of dynamic recovery. This is still only possible by assuming glide control.
It is demonstrated that the dislocation model can describe a range of properties without the use of adjustable parameters. These properties include secondary creep and stress-strain curves.